Three-dimensional colloidal crystals in liquid crystalline blue phases
Miha Ravnika,b, Gareth P. Alexanderb,c, Julia M. Yeomansb, and Slobodan Žumera,d,1
aFaculty of Mathematics and Physics, University of Ljubljana, 1000 Ljubljana, Slovenia; bRudolf Peierls Centre for Theoretical Physics, University of Oxford, Oxford OX1 3NP, United Kingdom; cDepartment of Physics and Astronomy, University of Pennsylvania, Philadelphia, PA 19104; and dJožef Stefan Institute, 1000 Ljubljana, Slovenia
Edited* by Noel A. Clark, University of Colorado at Boulder, Boulder, CO, and approved January 21, 2011 (received for review October 26, 2010)
Applications for photonic crystals and metamaterials put stringent using blue phases for colloidal assembly are (SI Text)(i) highly requirements on the characteristics of advanced optical materials, regular large-scale trapping potentials, (ii) strong potentials that demanding tunability, high Q factors, applicability in visible range, hold particles in trapping sites, (iii) simple control of the colloidal and large-scale self-assembly. Exploiting the interplay between crystal via restructuring of the liquid crystal under external fields, structural and optical properties, colloidal lattices embedded in and (iv) possible use of already developed assembly techniques liquid crystals (LCs) are promising candidates for such materials. from nonliquid crystal-based colloidal materials. Recently, stable two-dimensional colloidal configurations were Cubic blue phases (BPs) form in highly chiral liquid crystals demonstrated in nematic LCs. However, the question as to whether where rod-like molecules align in a periodic 3D orientational stable 3D colloidal structures can exist in an LC had remained texture with cubic symmetry (SI Text). Depending on tempera- unanswered. We show, by means of computer modeling, that col- ture, two distinct textures form, known as BP I and BP II. The loidal particles can self-assemble into stable, 3D, periodic structures texture of blue phases can be thought of as being made of stacked in blue phase LCs. The assembly is based on blue phases providing a cylindrical tubes—double-twist cylinders—where inside mole- 3D template of trapping sites for colloidal particles. The particle cules rotate to form helical vortices (Fig. S1) (23). In the space configuration is determined by the orientational order of the LC between cylinders molecular orientations cannot extend smoothly, molecules: Specifically, face-centered cubic colloidal crystals form forming a cubic lattice of defect lines, known as disclinations. in type-I blue phases, whereas body-centered crystals form in These places of molecular misalignment are the energetically type-II blue phases. For typical particle diameters (approximately most disfavored regions in blue phases. Placing particles within 100 nm) the effective binding energy can reach up to a few the disclinations replaces part of this energetically costly region k T 100 B , implying robustness against mechanical stress and tem- with the particles’ own volume, lowering the overall energy of perature fluctuations. Moreover, the colloidal particles substan- the LC texture. The reduction in energy is of order approximately tially increase the thermal stability range of the blue phases, for Kr, where K is an elastic constant and r is the particle radius, lead- a factor of two and more. The LC-supported colloidal structure k T ing to a binding energy of several hundred B for approximately is one or two orders of magnitude stronger bound than, e.g., 100 nm size colloids (24). Indeed, analogously, micron-sized par- water-based colloidal crystals. ticles were trapped in two spatial dimensions by a single disclina- ∣ ∣ ∣ tion in nematic (25, 26), polymer particles were trapped at the 3D self-assembly colloids chirality mesoscopic modeling defect boundaries of opposite twist domains (27), and recently stabilization of blue phases by nanoparticles (28, 29) and guest he major limitation of self-assembly approaches to building – components were demonstrated (30). T3D photonic materials (1 6) is the difficulty of scaling the The aim of this article is to show by phenomenological mod- materials up from the nanoscale to the device dimensions. The eling that colloidal particles can self-assemble into stable, 3D col- approaches typically rely on the manipulation of particles by loidal crystals in blue phase LCs. Three-dimensional colloidal van der Waals or screened electrostatic forces (7) and the manip- lattices are initialized according to the symmetry of intrinsic ulation proceeds either under ultra high vacuum conditions or in trapping sites in blue phases and then let to relax to equilibrium. water dispersions. The technological complexity lies in control- Several stable lattices with different total free energies per unit ling these forces over macroscopic length scales. Technologies cell are found in both BP I and II. The lattice with lowest free for 3D self-assembly are developed, based on electrically driven energy is face-centered cubic (FCC) in BP I and body-centered particle manipulation (8), sedimentation (9), growth on pat- cubic (BCC) in BP II. Interestingly, when doping blue phases with terned surfaces (10), tuning of electrostatic interactions between colloidal particles with weak surface of particle–liquid crystal oppositely charged particles (11, 12), and DNA-guided crystalli- interactions (i.e., weak surface anchoring), we find that the ther- zation (13). In liquid crystal colloids, the self-assembly is demon- strated for two-dimensional structures of clusters, chains, and mal stability range of blue phases increases substantially by a fac- two-dimensional crystals (14–17). There have been recent ad- tor of two or more. This increased thermal stability is explained vances in the synthesis and characterization of building blocks, by scaling analysis of the relevant contributions to the total free but these have not been matched by similar progress in organizing energy of blue phase colloids. the building blocks into assemblies and materials (18). Therefore, using cholesteric blue phases represents a unique and clear route Author contributions: M.R., G.P.A., J.M.Y., and S.Z. designed research; M.R. and G.P.A. to the 3D self-assembly of colloids. Recently, blue phases are performed research; M.R., G.P.A., J.M.Y., and S.Z. analyzed data; and M.R., G.P.A., receiving greater attention because materials with a broad stabi- J.M.Y., and S.Z. wrote the paper. lity range have been discovered (19, 20). In addition application The authors declare no conflict of interest. of a polymer-stabilized blue phase enabled development of a dis- *This Direct Submission article had a prearranged editor. play with a very fast response (21). Also, blue phases are attract- Freely available online through the PNAS open access option. ing broader attention because of growing interest in condensed See Commentary on page 5143. matter systems with analogous topological structures. One of the 1To whom correspondence should be addressed. E-mail: [email protected] more interesting topological structures are chiral ferromagnets This article contains supporting information online at www.pnas.org/lookup/suppl/ such as recently discussed MnSi (22). The main advantages of doi:10.1073/pnas.1015831108/-/DCSupplemental.
5188–5192 ∣ PNAS ∣ March 29, 2011 ∣ vol. 108 ∣ no. 13 www.pnas.org/cgi/doi/10.1073/pnas.1015831108 Downloaded by guest on September 27, 2021 Three-Dimensional Colloidal Crystals (SC) lattice will compete, possibly forming polydomains. Finally,
To identify the energetically favorable trapping sites we calculate we should stress that the free energy differences between various SEE COMMENTARY the free energy density using a mean field Landau–de Gennes lattices also depend on surface anchoring and on LC material approach (31). Indeed, a single defect line can generate trapping parameters, therefore a particular choice of materials may ener- potentials as strong as approximately 200 kT for 30 nm particles, getically favor another crystalline structure (Fig. 2 B and D). but also regular arrays of defect lines in chiral nematics (32). Fig. 1 Experimentally, our process to generate colloidal crystals cor- shows isosurfaces of constant free energy density (green) and the responds to forming particles in situ, which we propose could network of disclination lines (red) within each of the blue phase actually be achieved by phase separation of chiral nematic and unit cells. The free energy density is largest in the core regions the second component. Building on the work of Loudet et al of the defects and drops substantially within the double-twist in nematic phase (33), one could perform temperature quench regions. The positions of the maxima in the free energy density within the blue phase to trigger phase separation and form par- reflect the cubic symmetry of the blue phase texture, so that the ticles—droplets—of the second component, now ideally at the trapping potential for the colloids also reflects this symmetry optimal trapping sites. Such a process could avoid clustering allowing crystalline arrangements of colloids to form. and formation of irregular metastable structures, which is other- Stable 3D colloidal crystals in BP I and BP II are shown in wise typically observed when introducing particles into defect Fig. 2 A–D. For simplicity, we choose particles including spheri- structures of liquid crystal (24). Being able to control uniform cally symmetric homeotropic surface alignment. Structures vary dispersion of particles, an alternative to phase separation could in the number of particles per unit cell, and correspond to regular be to use isotropic to cholesteric transition, allowing particles to crystalline configurations that can be stabilized by the symmetry move only when the blue phase defect pattern is fully established. provided by the blue phase defect pattern. In all structures, Fluctuations of particles between effective trapping sites in the the particles are individually trapped to effective trapping sites. blue phase pattern could break the crystalline order of particles. The structures are built by positioning a given number of particles To address the role of fluctuations, free energy barriers between per unit cell (one, two, and four) into predetermined symmetric the trapping sites are calculated. They prove to be strongly ani- trapping sites identified from the free energy density profile of sotropic and have easy directions (with lowest increase in energy) the BPs, and then let to fully equilibrate with respect to the always along disclination lines. The height of energy barriers ∼10 k T particle positions, size of the unit cell, and texture of the BP. All increases with particle size and is for 50 nm particles B shifts of particles from the symmetric positions lead to an increase along easy directions in both BP I and BP II. For smaller particles in free energy confirming that the crystalline arrangements (approximately 10 nm), this height of the energy barriers indi- are energetically preferred. cates that thermal fluctuations can cause fluctuations in particle To identify the equilibrium lattice, free energies of various BP positions and also migration of particles along disclinations, colloidal crystals relative to the FCC (BP I) and BCC (BP II) are whereas for larger particles (approximately 100 nm), fluctuations shown in Fig. 3 A and B. Interestingly, in BP I, we find that the are insufficient to cause changes in the structure. Another me- arrangement with lowest free energy is the FCC crystal (Fig. 2A) chanism that could affect the regularity of colloidal crystals is for the majority of particle sizes (smaller than approximately clustering of multiple particles in a single trapping site. Perform- 100 nm) and BCC for larger particles. Qualitatively, one can ing the analysis in BP II, we compared the configuration to one explain this change by an effectively smaller filling fraction in trapping site crowded by two particles and conversely one empty BCC crystals, which at larger particle sizes allows for more effi- site, with the regular crystalline BCC structure. The crowded con- cient relaxation of liquid crystal deformation imposed by surface ∼10 k T figuration was found to have B higher free energy, imply- anchoring. In BP II, the energetically most favorable structure ing that such crowding is energetically not favorable, because is BCC colloidal crystal (Fig. 2C). The free energy differences particles cannot optimally cover the disclination regions. To per unit cell between various lattices are typically larger than relate our work to studies of entropy-driven depletion forces that ∼10 k T k T B in BP I and larger than a few B in BP II. In BP I are technologically commonly used to achieve aggregation and the relatively large energy differences indicate favoring of a single crowding, they are generically small when compared to liquid (FCC or BCC) lattice, whereas in BP II the BCC and single cubic crystalline effective elastic forces because in blue phase colloids the separation between particles is typically at the scale of par- A ticles (approximately 100 nm) and not liquid crystal molecules (approximately 0.1 nm) (34, 35). Finally, the particle aggregation can be affected by the particle–liquid crystal interfacial tension, yet this behavior is strongly dependent on the specific choice of materials. Our work is only relevant for materials that give total PHYSICS wetting at the surfaces of particles where the interfacial tension can be ignored. Namely, for totally wetted surfaces, the surface area and therefore the surface tension energy remain unchanged B no matter the positioning or aggregation of particles. However, for typical materials, an estimate of the surface tension energy 2 −15 2 Fs gives Fs ¼ 4πγr ∼ 10 J[γ ∼ 0.03 N∕m is typical surface tension of LCs (36) and r ∼ 50 nm is typical particle radius], which is in similar to characteristic liquid crystalline energies of blue phase unit cells (Materials and Methods). Therefore, sur- face tension can profoundly affect the particle aggregation. Fig. 4 A and B shows the free energy, relative to a colloid- free texture, as a function of the particle radius for a range of anchoring strengths W. When W is weak, W ≲ 10−5 Jm−2, the Fig. 1. Local free energy density profile. (A)BPI.(B) BP II. Isosurfaces of the free energy density are shown in green. Disclination lines are drawn in red as free energy is steadily reduced by increasing the particle size. isosurfaces of the nematic degree of order S ¼ 0.23 (BP I) and S ¼ 0.1 (BP II). In this regime, particles stabilize the BP texture. The effect is lar- Regions with the highest free energy density coincide with the centers of the gest for weak anchoring and relatively large particle radius, defect lines and represent the optimum location for colloidal inclusions. r ∼ 100 nm. When the surface anchoring is strong, the distortions
Ravnik et al. PNAS ∣ March 29, 2011 ∣ vol. 108 ∣ no. 13 ∣ 5189 Downloaded by guest on September 27, 2021 A C
Fig. 2. Three-dimensional BP colloidal crystals. (A) Energetically favorable FCC colloidal crystal in BP I, (B) stable colloidal crystals in BP I with simple cubic (SC) and BCC unit cell, (C) the most energetically favorable BCC colloidal crystal in BP II, and (D) stable colloidal crystals in BP II with SC and four particle configuration S ¼ 0 23 S ¼ 0 40 r ¼ 70 (4PC) unit cell. In BP I, disclination lines are drawn as isosurfaces of degree of order . ( bulk . ), particle radius is nm. In BP II, disclination lines S ¼ 0 1 S ¼ 0 26 r ¼ 50 2 × 2 × 2 are visualized as isosurfaces of . ( bulk . ), nm. In all cases unit cells have been shown to better illustrate the structure.
induced in the BP texture are substantial and the overall free as ΔV ∼ rðr − 2ξ~Þ, with a minimum for r ¼ ξ~ at particle sizes energy is increased by the addition of the particles. comparable to the disclination core size ξ~. The core size ξ~ is pro- Fig. 4 C and D shows how the unit cell size of BP colloidal portional to the nematic correlation length ξ, giving typi- crystals depends on the particle size. In both BPs, the unit cell cally ξ ∝ ξ~ ∼ 10 nm. shrinks for small particles and expands for larger particles, with a quadratic dependence fitting the numerical results well. This Increasing Thermodynamic Stability of Blue Phases behavior may be understood if we recall that the energetic cost The reduction in free energy afforded by immersing colloidal of the disclinations pushes the double-twist cylinders apart, mak- particles offers an appealing mechanism for increasing the ing the unit cell in a colloid-free BP larger than the chirality alone thermodynamic stability of BPs. In Fig. 5 we show the phase would prefer (37). The removal of part of this cost allows the diagram for colloidal blue phases, calculated numerically for double-twist cylinders to pack more closely, reducing the lattice 100 nm radius particles with weak homeotropic anchoring W ¼ 10−5 ∕ 2 constant. However, if the colloid radius r is larger than the effec- ( J m ) and taking FCC colloidal crystals in BP I – tive core of the disclination, it will force the double-twist cylinders and BCC colloidal crystals in BP II. The cholesteric colloidal further apart, and increase the size of the BP unit cells. Effec- BP I phase boundary was estimated using an undistorted choles- tively, these changes of the effective thickness of double-twist teric texture and hence corresponds to an absolute upper limit. cylinders cause the change in volume of the unit cell to scale The effect of particles is pronounced, yielding a significant increase in the stability of both BP II relative to BP I and of BP I relative to the cholesteric For example, for BP II with par- −1 ticles, at a typical inverse pitch of 1∕p0 ¼ 2 μm , the tempera- ture range increases by a factor of approximately three. The general change in free energy caused by the colloids may be understood from scaling arguments. Each colloid removes a portion of the disclination network proportional to its radius, leading to a free energy savings on the order of Kr. The surface anchoring leads to a free energy cost on the order of Wr2, giving a net change in the energy of ∼−aKr þ bWr2, where a and b are positive constants. However, the particles also affect the size of the BP unit cell giving a term associated with the work done, −pΔV, where p is an effective pressure for the change in volume ΔV ∼ rðr − 2ξ~Þ Fig. 3. Relative free energies of various crystalline lattices as functions of . The complete scaling of the free energy then ~ 2 particle radii relative to FCC lattice and BCC lattice in (A) BP I and (B)BP takes the form ΔF ¼ð−aK þ 2pcξÞr þðbW − pcÞr , where c is II, respectively. another positive constant, and this scaling is in good agreement
5190 ∣ www.pnas.org/cgi/doi/10.1073/pnas.1015831108 Ravnik et al. Downloaded by guest on September 27, 2021 AB continuously would also provide an isotropic expansion or con-
traction of the blue phase unit cell, with technological interest SEE COMMENTARY as a tunable resonator in lasing applications (39). Indeed, in com- parison to usual solid state resonators, liquid crystal-based micro- resonators have proven to exhibit large Q factors and two orders of magnitude larger tunability (40). Finally, we mention that the use of fluorescently labeled colloids could enable a means of directly studying the structure of the blue phases (41) and of fol- lowing the kinetics of textural rearrangements (42, 43) and blue phase rheology (44). The important step beyond our work is the kinetics of blue CD phase colloids, as the formation of perfect colloidal crystals will have to compete with random arrangements and possible phase separation into colloid-rich and colloid poor regions. In addition, it is a priori uncertain that a BP nucleating from an isotropic phase dispersed with colloids will form the same cubic lattices that it does in the absence of particles. Thus, there is ample motivation for studying the kinetic aspects of colloidal particles in BPs, addressing domain growth (45), possible thermal anneal- ing, and external fields assisted assembly. In summary, we have demonstrated that 3D colloidal crystals can be assembled in LC blue phases by using the free energy gain Fig. 4. Free energy profile for various particle sizes and anchoring strengths W in (A) BP I FCC colloidal crystals and (B) BP II BCC colloidal crystals. Relative of trapping the particles in the core regions of defect lines. The unit cell sizes for various particle sizes and anchoring strengths of (C) BP I FCC universality of this mechanism opens routes for self-assembly. colloidal crystal and (D) BP II BCC colloidal crystal. Particle radius r ¼ 0 corre- Equilibrium configurations of FCC colloidal crystals in BP I and sponds to BP with no particles. Free energy and relative cell size profiles for BCC colloidal crystals in BP II were identified as being energe- −6 2 W ¼ 10 J∕m change for less than 2% and 0.01%, respectively, upon tically most favorable. The effects of particle size and surface W → 0 further decreasing the anchoring strength ( ). anchoring properties were addressed, as main material tunability parameters. Two specific roles were identified: Colloidal particles with the numerical results in Fig. 2. By optimizing the regime with weak surface anchoring increase the thermodynamic stability ΔF of negative , one maximizes the phase stabilization of blue of BPs and larger particles and stronger surface anchoring give phases. stronger binding of particles to the trapping sites in BPs. How- Discussion ever, both the size of particles and surface anchoring affect To stabilize the blue phases, we expect it to be energetically the 3D profile of 3D trapping sites, which can change the relative favorable to use numerous small (nano-sized) particles, as they metastability of various possible particle lattices. In a wider con- can more effectively fill the defect cores and reduce the total free text, our results open a unique direction for the assembly of com- energy. Even more effective filling of the defects could be plex 3D optical structures and their possible application in achieved by using anisotropic particles, e.g., ellipsoids or spher- photonics and plasmonics. Moreover, ordering and stabilization ocylinders. As the relative metastability of the different crystal- of complex chiral spatial 3D fields bring our results in close line structures is dependent on particle size, an interesting relation to other chiral condensed matter systems, including approach would be to use electro- or thermo-responsive particles skyrmions and superconductive vortices. (38), which may allow for a reconfiguration of the crystalline Materials and Methods structures by continuously changing the particle size. Based on To model blue phase colloids, we employ a continuum, mean field Landau– the free energy profile of BP II (Fig. 1B), we speculate that the de Gennes approach based upon the tensor order parameter, Qij. This body-centered cubic configuration (Fig. 2C) could transform into approach naturally accounts for effective elasticity of the liquid crystal, var- the four particle configuration (Fig. 2D, Right) upon reducing iations in the magnitude of the order, and possible biaxiality. The free energy the size of the particles. Furthermore, changing the particle size is taken to be PHYSICS
Fig. 5. BP phase stabilization by particle doping. (Left) Phase diagram of BP colloidal crystals in terms of inverse cholesteric pitch 1∕p0 and temperature T T ( IC is isotropic-cholesteric transition temperature). Red lines are phase boundaries of the BP with immersed colloidal particles (homeotropic anchoring −4 2 W 0 ¼ 10 J∕m ). Black lines show phase boundaries of the chiral LC with no particles. Note the large increase in the phase space of the BP region when particles are introduced. (Right) Shows examples of corresponding BP colloidal crystals at specific temperature and inverse pitch.
Ravnik et al. PNAS ∣ March 29, 2011 ∣ vol. 108 ∣ no. 13 ∣ 5191 Downloaded by guest on September 27, 2021 Z A ð1 − γ∕3Þ A γ A γ We obtained minimum energy configurations by solving a system of F ¼ 0 Q Q − 0 Q Q Q þ 0 ðQ Q Þ2 V 2 ij ij 3 ij jk ki 4 ij ij d coupled partial differential equations with appropriate boundary conditions LCZ using an explicit Euler finite difference relaxation algorithm on a cubic mesh. L ∂Q ∂Q ∂Q To produce the desired blue phase texture, initial conditions were chosen for þ ij ij þ 2q Lϵ Q lj V 0 ikl ij d the tensor Qij corresponding to analytic expressions in the high chirality limit LC 2 ∂xk ∂xk ∂xk Z (q0 → ∞). The surface of each particle is defined by the set of mesh points W þ ðQ − Q0ÞðQ − Q0Þ S;  contained within a spherical shell with thickness equal to the mesh resolu- ij ij ij ij d tion. Mesh points outside the surface are updated according to the bulk CS 2 Ginzburg–Landau equations, appropriate boundary conditions are imposed on the surface points and no computations are performed for the interior where LC denotes an integral over the volume occupied by the liquid crystal points. For computational efficiency, the effects of fluid flow are neglected only and colloidal surfaces (CS) over the surfaces of the colloidal particles. in the relaxational dynamics as these are not expected to effect the equili- The first term is the bulk free energy and describes a first order transition brium configurations. (at γ ¼ 2.7) between an isotropic and a nematic phase, with A0 a constant Material parameters were chosen to match a typical cholesteric nematic with the dimensions of an energy density and γ an effective dimensionless liquid crystal and, if not stated differently, were taken to be: L ¼ 2.5× temperature. The second term describes the energy cost of distortions in the −11 5 3 −4 2 10 N, A0 ¼ 1.02 × 10 J∕m , W ¼ 10 J∕m ,(γ ¼ 3.375, p0 ¼ 0.566 μm) in liquid crystalline order; L is an elastic constant, q0 is a chiral parameter related BP I, and (γ ¼ 2.755, p0 ¼ 0.616 μm) in BP II. to the pitch of the cholesteric helix by p ¼ 2π∕q0 and ϵikl is the fully anti- symmetric alternating tensor equal to þ1ð−1Þ if i, k, l is an even (odd) per- mutation of one, two, three, and zero otherwise. The final term describes the ACKNOWLEDGMENTS. M.R. acknowledges support of the European Commission (EC) under the Marie Curie Program Active Liquid Crystal Colloids, content interaction of the liquid crystal with the surfaces of the colloids, where W Q0 reflects only the authors views and not the views of the EC. G.P.A. thanks Randall represents the strength of the surface anchoring and ij is the order para- Kamien for discussions and acknowledges funding from National Science meter preferred by the surface, which we take to be homeotropic. The equi- Foundation Grant DMR05-47320. M.R. and S.Z. acknowledge funding from librium surface and bulk profile of the order parameter tensor is qualitatively Slovenian Research Agency P1-0099, J1-2335, FP7 215851-2 Hierarchy, and unchanged in the most relevant regime of weak anchoring. Center of Excellence Advanced Materials and Technologies for the Future.
1. Hellweg T (2009) Towards large-scale photonic crystals with tuneable band gaps. 25. Pires D, Fleury J-B, Galerne Y (2007) Colloid particles in the interaction field of a Angew Chem Int Ed 48:6777–6778. disclination line in a nematic phase. Phys Rev Lett 98:247801. 2. Hornreich RM, Shtrikman S, Sommers C (1994) Photonic band gaps in body-centered- 26. Fleury J-B, Pires D, Galerne Y (2009) Self-connected 3-D architecture of microwires. cubic structures. Phys Rev B: Condens Matter Mater Phys 49:10914–10917. Phys Rev Lett 103:267801. 3. Tanaka Y, et al. (2007) Dynamic control of the Q factor in a photonic crystal nanocavity. 27. Voloschenko D, et al. (2002) Effect of director distortions on morphologies of phase Nat Mater 6:862–865. separation in liquid crystals. Phys Rev E: Stat Nonlinear Soft Matter Phys 65:060701(R). 4. Yao J, et al. (2008) Optical negative refraction in bulk metamaterials of nanowires. 28. Yoshida H, et al. (2009) Nanoparticle-stabilized cholesteric blue phases. Appl Phys Science 321:930–930. Express 2:121501. 5. Won R (2009) Photonic crystals on a chip. Nat Photonics 3:498–499. 29. Karatairi E, et al. (2010) Nanoparticle-induced widening of the temperature range of 6. Kang D, et al. (2001) Electro-optic behavior of liquid-crystal-filled silica opal photonic liquid-crystalline blue phases. Phys Rev E: Stat Nonlinear Soft Matter Phys 81:041703. – crystals: Effect of liquid-crystal alignment. Phys Rev Lett 86:4052 4055. 30. Fukuda J (2010) Stabilization of a blue phase by a guest component: An approach 7. Israelachvili JN (2011) Intermolecular and Surface Forces (Elsevier, Oxford). based on a Landaude Gennes theory. Phys Rev E: Stat Nonlinear Soft Matter Phys 8. Pishnyak OP, et al. (2007) Levitation, lift, and bidirectional motion of colloidal particles 82:061702. in an electrically driven nematic liquid crystal. Phys Rev Lett 99:127802. 31. Alexander GP, Yeomans JM (2006) Stabilizing the blue phases. Phys Rev E: Stat 9. Miguez H, et al. (1998) Control of the photonic crystal properties of fcc packed Nonlinear Soft Matter Phys 74:061706. – submicrometric SiO2 spheres by sintering. Adv Mater 10:480 483. 32. Ravnik M, Alexander GP, Yeomans JM, Zumer S (2010) Mesoscopic modelling of 10. Van Blaaderen A, Ruel R, Wiltzius P (1997) Template-directed colloidal crystallization. colloids in chiral nematics. Faraday Discuss 144:159–169. Nature 385:321–324. 33. Loudet J-C, Barois P, Poulin P (2000) Colloidal ordering from phase separation in a 11. Leunissen ME, et al. (2005) Ionic colloidal crystals of oppositely charged particles. liquidcrystalline continuous phase. Nature 407:611–613. Nature 437:235–240. 34. Kaplan PD, Faucheux LP, Libchaber AJ (1994) Direct observation of the entropic 12. Hynninen A-P, Thijssen JHJ, Vermolen ECM, Dijkstra M, Van Blaaderen A (2007) Self- potential in a binary suspension. Phys Rev Lett 73:2793–2796. assembly route for photonic crystals with a bandgap in the visible region. Nat Mater 35. Roth R, Evans R, Dietrich S (2000) Depletion potential in hard-sphere mixtures: Theory 6:202–205. and applications. Phys Rev E: Stat Nonlinear Soft Matter Phys 62:5360–5377. 13. Nykypanchuk D, Maye MM, van der Lelie D, Gang O (2008) DNA-guided crystallization 36. Gannon MGJ, Faber TE (1978) The surface tension of nematic liquid crystals. Philos of colloidal nanoparticles. Nature 451:549–552. Mag A 37:117–135. 14. Poulin P, Stark H, Lubensky TC, Weitz DA (1997) Novel colloidal interactions in 37. Grebel H, Hornreich RM, Shtrikman S (1983) Landau theory of cholesteric blue phases. anisotropic fluids. Science 275:1770–1773. Phys Rev A: At Mol Opt Phys 28:1114–1138. 15. Yada M, Yamamoto J, Yokoyama H (2004) Direct observation of anisotropic interpar- 38. Debord SB, Lyon LA (2003) Influence of particle volume fraction on packing in respon- ticle forces in nematic colloids with optical tweezers. Phys Rev Lett 92:185501. – 16. Ravnik M, et al. (2007) Entangled nematic colloidal dimers and wires. Phys Rev Lett sive hydrogel colloidal crystals. J Phys Chem B 107:2927 2932. ń 99:247801. 39. Cao W, Mu oz A, Palffy-Muhoray P, Taheri B (2002) Lasing in a three-dimensional – 17. Musevic I, et al. (2006) Two-dimensional nematic colloidal crystals self-assembled by photonic crystal of the liquid crystal blue phase II. Nat Mater 1:111 113. topological defects. Science 313:954–958. 40. Humar M, Ravnik M, Pajk S, Musevic I (2009) Electrically tunable liquid crystal optical – 18. Min Y, Akbulut M, Kristiansen K, Golan Y, Israelachvili J (2008) The role of interparticle microresonators. Nat Photonics 3:595 600. and external forces in nanoparticle assembly. Nat Mater 7:527–538. 41. Higashiguchi K, Yasui K, Kikuchi H (2008) Direct observation of polymer-stabilized 19. Coles HJ, Pivnenko MN (2005) Liquid crystal “blue phases” with a wide temperature blue phase I structure with confocal laser scanning microscope. J Am Chem Soc range. Nature 436:997–1000. 130:6236–6327. 20. Castles F, Morris SM, Terentjev EM, Coles HJ (2010) Thermodynamically stable blue 42. Kitzerow H-S (1991) The effect of electric fields on blue phases. Mol Cryst Liq Cryst phases. Phys Rev Lett 104:157801. 202:51–83. 21. Kikuchi H, Yokota M, Hisakado Y, Yang H, Kajiyama T (2002) Polymer-stabilized liquid 43. Alexander GP, Marenduzzo D (2008) Cubic blue phases in electric fields. Europhys Lett crystal blue phases. Nat Mater 1:64–68. 81:66004. 22. Muhlbauer S, et al. (2009) Skyrmion lattice in a chiral magnet. Science 323:915–919. 44. Dupuis A, Marenduzzo D, Orlandini E, Yeomans JM (2005) Rheology of cholesteric blue 23. Wright DC, Mermin ND (1989) Crystalline liquids—the blue phases. Rev Mod Phys phases. Phys Rev Lett 95:097801. 61:385–432. 45. Henrich O, Stratford K, Marenduzzo D, Cates ME (2010) Ordering dynamics of blue 24. Zapotocky M, et al. (1999) Particle-stabilized defect gel in cholesteric liquid crystals. phases entails kinetic stabilization of amorphous networks. Proc Natl Acad Sci USA Science 283:209–212. 107:13212–13215.
5192 ∣ www.pnas.org/cgi/doi/10.1073/pnas.1015831108 Ravnik et al. Downloaded by guest on September 27, 2021